For coated surfaces:
- In good condition: Wash down with a suitable detergent, rinse with fresh water and allow to dry. Abrade with 280320 grade (grit) paper.
- In poor condition: Remove all previous coatings and prime the surface.
All surfaces: Sand primer with 180-220 grit. Afterwards, remove dust residues from the surface and apply 1-2 coats of Interdeck.
Bare wood: Abrade with 80-180 grit sandpaper. Then with 280 grit paper. Remove sanding dust by brushing, dusting and wiping. Allow to dry completely.
Aluminium: : Degrease with solvent or Super Cleaner. Sand well using 24120 grade (aluminium compatible) paper. Clean thoroughly and allow to dry. Prime with One UP as soon as possible (within 8 hours).
Steel: Degrease with solvent or Super Cleaner.Gritblast to Sa 2½ near white metal surface. If gritblasting is not possible, grind the metal surface with 2436 grit abrasive discs to a uniform, clean, bright well roughened metal surface (5075microns) anchor pattern. Use angle grinder on small areas. Clean thoroughly and allow to dry and then apply primer.
GRP: Degrease with solvent or Super Cleaner. Sand well using 180220 grade paper. Clean thoroughly and allow to dry and apply primer.
Old / weathered gelcoat:Degrease with thinner or Super Cleaner. Thoroughly sand with 180-220 grit sandpaper. Clean well and allow to dry. To prevent blistering, apply 3 coats of a 2-component primer, then overcoat with a 2-component undercoat.
Drying time at 15 °C: 4 hours
Processing time at 15 °C: min. 20 hours
Processing temperature: +5 °C to max. 35 °C
Please note the following hazard warnings:
Klanten kopen ook
Customers ask customers
Your question will be automatically forwarded to other SVB customers and your question will be published on the product page. Please do not pose any questions which can only be answered by the SVB team – such as the status of an order or product availability. You are also more than welcome to contact our SVB team by email at: firstname.lastname@example.org or by phone at: +49 (0)421-57290-0 .